Full Terms & Conditions of access and use can be found at
Download by: [Firat Universitesi] Date: 21 November 2017, At:
Journal of Civil Engineering and Management
ISSN: 1392-3730 (Print) 1822-3605 (Online) Journal homepage:
Effects of graphite on mechanical properties of stone mastic
Baha Vural Kök, Mehmet Yilmaz & Yunus Erkus
To cite this article: Baha Vural Kök, Mehmet Yilmaz & Yunus
Erkus (2017) Effects of graphite on mechanical properties of stone
mastic asphalt pavement, Journal of Civil Engineering and
Management, 23:8, 1013-1020, DOI:
To link to this article:
Published online: 20 Nov 2017.
Submit your article to this journal
View related articles
View Crossmark data
2017 Volume 23(8): 1013–1020
1013 Copyright © 2017 Vilnius Gediminas Technical University (VGTU)
EFFECTS OF GRAPHITE ON MECHANICAL PROPERTIES OF STONE MASTIC
Baha Vural KÖKa, Mehmet YILMAZa, Yunus ERKUSb
aDepartment of Civil Engineering, Engineering Faculty, Frat
University, 23100, Elaz, Turkey bDepartment of Civil Engineering,
Technology Faculty, Frat University, 23100, Elaz, Turkey
Received 19 Apr 2017; accepted 07 Jul 2017
Abstract. Hot mix asphalt needs to be developed to resist
particular permanent deformations like rutting and thermal cracking
due to increased traffic volumes and vehicle loads. Additives such
as carbon black, graphite, carbon fibers are used in the mixture or
the binder for improving the mechanical features of asphalt. In
this article, the effects of graphite used for developing the
mechanical properties of asphalt have been investigated in mixtures
tests. Therefore, Marshall stability, indirect tensile stiffness
modulus and indirect tensile fatigue tests were performed to
bituminous mixtures modified with three different proportions of
graphite by weight of bitumen. Stone mastic asphalt mixtures which
were manufactured with pure and modified bitumen were aged in
different time intervals in the oven. In conclusion, it has defined
that Marshall stability values have declined. It has been
determined that there is no significant difference in the
time-dependent deformation behavior of the original and aged
samples in pure and different graphite content although the
stiffness modulus and load repeat number of the samples increased
with the rise of the aging time. These results shown that graphite
generally used for improving the thermal properties in literature
were also determined to contribute to mechanical properties of
mixtures. Keywords: graphite, stone mastic asphalt, aging,
mechanical properties, bitumen, pavement.
Large parts of transport in the world are made with high- ways and
heavy traffic increases day by day thereby the roads are
structurally damaged. Heavy vehicle traffic and overmuch load
repetition, as well as environmen- tal factors, cause major
disruptions on the roads. There are various ways of preventing
these disruptions. One of these ways is to obtain more powerful
mixtures by changing the aggregate gradation (Liu et al. 2012). In
practice, the most obvious example of this is stone mas- tic
asphalt (SMA). Using of stone mastic asphalt earns high durability,
low permeability, low traffic noise pol- lution, high strength
against reflective cracks and high strength against rutting
properties to asphalt layer in the road (Austroads Technical Report
2002). It was also de- termined that elastic property of SMA could
be improved by adding waste polyethylene terephthalate and styrene-
butadiene-styrene (Moghaddam et al. 2012; Mokhtari, Nejad 2012).
Another way to prevent of these distortions is to modify the
bitumen. Due to viscoelastic behavior of bituminous binder,
mechanical features of asphalt pave- ment vary significantly
because of daily and seasonal temperature changes. Asphalt concrete
temperature can ascend to 70 °C in summer owing to it’s over
tion parameter (Van Bijsterveld et al. 2001). Further- more, this
incident eventually deteriorates the durability of pavement. It
will trigger the permanent deformations of pavement with the impact
of loads (Tongyan et al. 2012). It was determined that thermal
expansion were slightly larger than the thermal contraction
(Mamlouk et al. 2005) There are various ways to prevent deteriora-
tions occurred from high temperatures in the pavement. One of them
is the use of thermally conductive materi- als in order to improve
the resistance of pavement to the adverse effect of high
temperature. Du and Wang (2015) showed that using graphite in
asphalt mixture can suc- cessfully transmit the temperature to the
bottom layers. It was determined that the temperature decreased 6.5
°C at the 4 cm depth from the surface which induced 43.5% decrease
in rutting by using graphite as an additive. Liu et al. (2014)
determined that using 40% graphite with 0.3% carbon fiber induces
78%, 15% and 4% increase in dynamic modulus, indirect tensile
strength and Marshall stability of the bituminous mixtures
respectively. Lu et al. (2008) produced conductive asphalt concrete
using steel slag as aggregate and graphite in bituminous mixtures.
They have concluded that Marshall stability and dynamic
1014 B. V. Kök et al. Effects of graphite on mechanical properties
of stone mastic asphalt pavement
stability values of mixtures declined a bit with the rise of
graphite percentage, but these mechanical properties values still
compensate the standard requirements. The authors recommended
constructing thermal-modified pavement structure in order to
improve the rutting and fatigue cracking resistance (Chen et al.
Another important issue about the deterioration of bituminous
mixture is aging processes. Firstly the bitu- men used asphalt
mixtures are subjected to short-term aging during production and
paving processes and then exposed to long-term aging throughout
service life. The chemical change due to oxidation results in a
harder, more brittle asphalt mixture, which induces low temper-
ature cracking, fatigue cracking or another mode of dis- tress. It
was determined that mixing time has an effect on the mechanical
properties of SMA during the production. It was also stated that
different batching technologies impact an unstable bitumen
short-term aging (Brainas et al. 2013). Researchers have been
studying on mitigat- ing the adverse effects of aging by using
various addi- tives and also investigates new technics to evaluate
the aging processes. Warm-mix-asphalt additives which in- duced a
reduction in mixing and compaction temperature was reported to be
used successfully for the stone mastic asphalt (Kim et al. 2015).
The influence of the additives especially after long-term aging
should be observed in order to make a comprehensive evaluation
about the ser- vice life of hot mixtures. It was determined that
aging induces more stiffness for the unmodified mixtures than for
polymer or rubber modified mixtures (Radziszewski 2007). Wang et
al. (2015) showed that Styrene-butadi- ene-styrene (SBS) which is a
widely used binder additive and significantly contribute to the
performance of unaged binder may lose its modifying function after
long-time aging. FT paraffin wax was found to be effective in en-
hancing the resistance to aging (Aghazadeh Dokandari et al. 2014).
The improvement effects of crumb rubber on short-term aging
properties of asphalt binder are re- ported by the researchers
(Dong, Tan 2011; Reed 2010; Shatnawi 2012). Conversely it was
determined that the asphalt binder source rather than the
nanoparticle content plays an important role in determining the
influence of long-term ageing process (Xiao et al. 2011). In
another study, the thermal properties of graphite added binders are
examined. It is found that graphite improves the anti- aging
properties of the bitumen (Pan et al. 2014). Yao
et al. (2016) investigated the effects of 1–2% graphite
nanoplatelets on asphalt binder properties. It was deter- mined
that aging groups increases in the graphite modi- fied binder which
results in an increased resistance to rutting and moisture damage.
Graphite nanoplatelets also improve the resistance to
Although there are some studies about the thermal properties of
bituminous mixtures containing graphite, there are limited studies
about the effect of graphite on mechanical properties of stone
mastic asphalt mixtures. In this study, the effects of the
different amount of graph- ite on the mechanical properties of
mixtures were inves- tigated in large-scale.
1. Materials In this article, the aggregate and the filler used to
manu- facture of the asphalt mixtures are chosen as the lime-
stone. The bitumen (B 50/70) supplied from TÜPRA refinery was
utilized for the produce of modified bind- ers. The properties of
the bitumen are given in Table 1. Graphite powder passing the No.
200 sieve (0.075 mm) has a carbon content of 85.7%, an electrical
resistivity of 10–4 .m and a density of about 2.15 g/cm3. Elemental
analysis of graphite used in bitumen modification is given in Table
2. SEM image of graphite powder is also shown in Figure 1. In the
mixture samples, the limestone’s ag- gregate characteristics were
given in Table 3 was used.
2. Test sample preparation Bituminous hot mixture samples were
prepared as stone mastic asphalt, which has high resistance to the
Table 2. The elemental analysis of the graphite
Table 3. Physical properties of aggregate
Properties Standard Limits Coarse Fine Filler Abrasion loss (%)
(Los Angeles) ASTM C 131 (2014) Max 30 25 – – Frost action (%)
(Na2SO4) ASTM C 88 (2013) Max 10 4.5 – – Flat and elongated
particle (%) ASTM D 4791 (2010) Max 10 4 – Water absorbtion (%)
ASTM C127 (2015) Max 2 1.37 – Specific gravity (Gsb) ASTM C127
(2015) 2.613 – – Specific gravity (Gsb) ASTM C128 (2015) – 2.622 –
Specific gravity (Gsa) ASTM D854 (2014) – – 2.711
Table 1. The properties of the bitumen
Properties Value Penetration (25 °C, 100 g, 5 s, 0.1 mm) 51.2
Softening point (°C) 52.2 Penetration indeks –0.6 Density (g/cm3)
1.013 Viscosity (cP, 135 °C) 600 Viscosity (cP, 165 °C) 175
Journal of Civil Engineering and Management, 2017, 23(8): 1013–1020
has a high durability due to the high bitumen content and has
recently been widely used in high standard roads. Gradation
prepared according to Turkish Highway Tech- nical Specification
stone mastic wear layer Type-1 is shown in Table 4 and was designed
in accordance with standard Marshall design method. In order to
compare the effects of graphite powder on mechanical performance of
asphalt mixture, all the mixture samples were prepared with the
same gradation and same asphalt content.
Table 4. The gradation of the stone mastic asphalt
Sieve size (mm) 19 12.5 9.5 4.75 2.0 0.425 0.180 0.075
Passing (%) 100 95 62.5 37.5 25 17 13 10
Asphalt binder (500±5 g) was firstly heated to 165±5 °C in the
container. Then, graphite was added gingerly within 10 min, while
the shear speed was kept at 1000 rpm. Hot mix asphalt samples were
prepared with the bituminous binders. Graphite was added into pure
bitumen in 3 different ratios as 10%, 15% and 20% by weight of
bitumen used in mixtures and they were represented as 0% (G0), 10%
(G10), 15% (G15) and 20% (G20), respectively. The stone mastic
asphalt mixtures obtained with pure and modified binders were aged
for 1, 2 and 3 weeks in the oven at 50 °C. In the study totally 4
different mixtures were evaluated with aging. The effects of
graphite on mixture’s properties were examined by Marshall
stability, indirect tensile fatigue and indirect tensile stiffness
modulus tests with cylindrical shape specimens prepared 101 mm
diameter and 65 mm height.
3. Test methods
3.1. Marshall stability test Marshall stability test on hot mix
asphalt specimen was applied according to TS EN 12697-34 (2004).
Stability is described as the maximum strength against deforma-
tion. Flow is also the vertical deformation that occurs in time
which reaches the maximum load of the sample in the standard. The
samples were stored in a water bath at 60±1 °C for 40 minutes. The
samples were loaded at a speed of 50±2 mm/min. In the experiment,
the maximum load and deformation occurred at the maximum load were
3.2. Indirect tensile stiffness modulus test The stiffness modulus
which is a measure of the load distribution capability of
bituminous pavement is one of the most important performance
characteristics of bituminous hot mixtures (Zoorob, Suparma 2000).
The indirect tensile stiffness modulus (ITSM) test, a non-de-
structive and deformation-controlled test, described in BS DD
213:1993 standard and it is carried out by using the UMATTA
(Universal Material Testing Apparatus). The test apparatus are
shown in Figure 2. The test was car- ried out at 20 °C. Before the
experiment, the samples were kept at the test temperature for at
least 3 hours. The values such as sample height, diameter,
estimated Poisson ratio (0.35), target horizontal deformation (6.5
µm), load application time (3000 ms) and load rise (124 ms) times
were entered the software. ITSM values Sm (MPa) were calculated
according to following formula:
Sm = F(R + 0.27) / LH, (1)
where F is the maximum vertical load (N); H is the aver- age
horizontal deformation (μm) occurring after 5 load repetition; L is
the average sample thickness (mm) and the R is the Poisson ratio
3.3. Indirect tensile fatigue test The bituminous materials used on
the roads are exposed to a short time load during the passage of
Fig. 1. SEM image of graphite
Fig. 2. The indirect tensile stiffness modulus test apparatus
1016 B. V. Kök et al. Effects of graphite on mechanical properties
of stone mastic asphalt pavement
These loads lead to micro-damage which reduces the ri- gidity of
the material. These micro- damages cause pave- ment deterioration
called fatigue cracks in long-term (Francken 1998). Fatigue cracks
commonly occurred at bituminous hot mixtures, are the type of
deterioration caused by the load. Fatigue cracks are gradually
increas- ing by following the formation of the crack with repeti-
tive loads. The cylindrical test specimens are applied to repeated
pressure loads in the vertical diametric plane. This loading
creates tensile stresses relatively uniform in the horizontal
diametrical direction and vertical to the ap- plied load direction.
The tensile stresses cause to split in the middle at the vertical
direction of the specimen. The test apparatus are shown in Figure
3. The test was car- ried out at stress controlled condition by
applying cyclic constant loads of 350 kPa with a 0.1-s loading
followed by a 1.4-s rest period. The test was carried out at 20 °C.
The experiment continued until the specimens completely
4. Results and discussions
4.1. Marshall stability test results Marshall specimens were
prepared by applying 50 blow on both sides due to determine the
optimum bitumen ratio of the asphalt mixtures prepared with the
pure binder. The bituminous content was selected with 0.5%
increments from 5% to 7%. The fiber which is used for stabilizing
the high amount of binder was used as 0.5% by weight of the
mixture. The volumetric properties such as bulk specific gravity
(Gmb), air void (Va), voids in mineral aggregate (VMA), voids
filled with asphalt (Vfa) and the stability-flow values of the
samples prepared in different bitumen contents were determined. The
optimum bitu- minous content of the pure mixture was determined as
6.5%. The graphite-added samples were prepared in the same bitumen
content. The average values of the char- acteristics of all samples
with 6.5% bitumen content are given in Table 5. It was found that
Marshall stability val- ues declined with the increasing of
graphite content. This reduction can be thought to be due to the
oily properties of graphite. The maximum usage of graphite (20%)
in- duces only 6% reduction in stability. All of the mixtures
provide the minimum VMA and air voids requirements which are 16%
and 3–4% respectively. Stone mastic as- phalt mixtures give high
flow values compared to dense graded mixtures. An example of a
is given in Figure 4 (Kok et al. 2014). As it is seen here that SMA
mixtures hold the load in its body longer than that of the dense
graded mixtures due to having a coarse gradation. Therefore SMA
mixtures do not show a peak stability value, it bears the load
longer than the dense grad- ed mixture in the meantime it exhibits
high flow values.
4.2. Indirect tensile stiffness modulus test results For this
experiment, three samples were prepared for each sample type. Each
sample was subjected to loading at three different locations and 9
values were obtained for a sample type. ITSM values were determined
by calculat- ing the averages of the seven values outside the
largest and the smallest of these values. The test was carried out
at 20 ºC with deformation control. The target deformation was set
to 6.5 microns.
Fig. 3. The indirect tensile fatigue test apparatus
Fig. 4. The stability-flow curves of SMA and dense graded asphalt
(Kok et al. 2014)
Table 5. The average values of the characteristics of the
Specimen Type Gmb Va
Journal of Civil Engineering and Management, 2017, 23(8): 1013–1020
At first, the deformation-time characteristics of the specimens
were examined. The deformation-time relation of the original and
aged samples is given for pure and 20% graphite added samples in
Figure 5. At the repre- sentation of the specimen the first number
indicate the graphite content and the second one presents the aging
time in a week. G20-3 stand for 20% graphite added sam- ples aged 3
weeks at 50 °C in the oven. It is seen from the figures that the
deformations return since the load is removed after the sample
reaches to the maximum target deformation at about 150
milliseconds. It was determined that the deformations at 400th
milliseconds are between 2 and 3 microns in all graphite contents.
Even at the high- est graphite level (20%), there is no significant
difference either positively or negatively in the elasticity
properties compared to the pure mixture. The effects of aging time
on deformation characteristics do not so important for both pure
and graphite added mixtures.
The area under the stress-deformation curves is con- sidered as a
measure of the load distribution capability of the sample.
Stress-deformation relations of the unaged and three-week aged
specimens are given as depending on the graphite due to see the
effects of the graphite rate on the areas in Figure 6. While there
is no significant difference between the unaged pure and graphite
added samples, 20% graphite added mixture exhibits different
performance compared to others after the three-week ag- ing
conditions. Since this test is performed at elastic re- gion by
considering the 6.5 deformations as target defor- mation, it
enables to compare the flexibility properties of the samples in the
linear viscoelastic region. In this
respect, it can be concluded that the graphite added mix- tures up
to 15% graphite content do not have a significant performance
compared to the pure mixture. Besides the high amount of graphite
(20%) take effect after 3-week aging conditions.
Figure 7 shows the effect of aging time on the stress- deformation
relation of pure and G20 mixtures. It is seen that the areas under
the curves change at a considerable degree depending on the aging
period. In all samples, it was determined that the areas rise with
the increase of the aging time indicating an improved ability to
absorb the elastic energy, at medium temperatures.
Stiffness modulus (Sm) of all mixtures types in all aging
conditions are given in Figure 8. It is seen that graphite content
does not have any influence on stiffness modulus at the unaged
condition. Pure and 10% graphite added mixtures exhibit similar
performance at all aging time. Sm values of these mixtures increase
gradually with the aging time. However, the mixtures show different
per- formance after 15% graphite content depending on the aging
time. The aging time loses its significance for the 15% and 20%
graphite added mixtures. The Sm values of the G15 and G20 mixtures
after 1, 2 and 3 weeks are close to each other but 49–58% higher
than that of the unaged ones. 20% graphite content also induces 44%
in- crement in the Sm values of the pure mixture.
4.3. Indirect tensile fatigue test results In the fatigue test,
three samples experimented to each type of mixture. The load
repetition number – deforma- tion relations of the pure and 20%
Fig. 5. The deformation-time relation of the asphalt mixtures Fig.
6. The stress-deformation relation of the asphalt mixtures with
1018 B. V. Kök et al. Effects of graphite on mechanical properties
of stone mastic asphalt pavement
mens at different aging times are given in Figure 9. These curves
belong to a nearest average of the three samples tested for each
type of mixture. As it can be seen from the figures, all samples
show a rapid deformation at the beginning and the increase of
deformation trend contin- ues linearly and then increases rapidly
again. The rapid deformation increase of the curves at the
beginning is caused by the decreasing of the air volume due to com-
pression in the samples. The specimens exhibit elastic behavior for
certain time by inducing a linear increase in deformations. After
the initial crack in the specimen, the deformation increase
accelerates again. In the phase after the beginning of the crack,
which is called as the third region in the pure mixture, it is seen
that the samples do not take up much load and break even before
reaching the third region. In graphite-added samples, the third
region is obviously formed. In other words, after the
of the crack, the graphite-added specimens show more resistance to
the progress of the crack.
The load repetition number of all sample types in- creases
significantly with the increase of aging time. Since the samples
were collapsed at different deformation levels, 4 mm deformation
was selected as the threshold value, which is the lowest
deformation level reached by all samples in order to make a correct
comparison be- tween them. The average load repetition numbers of
the specimens at 4 mm deformation are given Figure 10. The figure
provides for assessing the aging effect on mixture by considering
the slope of the curves. Pure and G10 mixtures have the lowest
slope, G15 and G20 have the highest. Effects of aging time on load
repetition number is more pronounced after the 15% graphite
content. G10, G15 and G20 mixtures have 7%, 65% and 78% higher load
repetition number compared to the pure mixture af- ter 3-week aging
Fig. 7. The stress-deformation relation of the asphalt mixtures
Fig. 8. The stiffness modulus (Sm) values of mixtures in aging
Fig. 9. The load repetition number-deformation relation of the
mixtures with aging
Fig. 10. The load repetition numbers of the mixtures at 4 mm
Journal of Civil Engineering and Management, 2017, 23(8): 1013–1020
The deformation-load repetition number relationship of samples in
the different graphite contents is given Fig- ure 11 for the unaged
and 3-week aged conditions. The graphite content in the unaged
samples has no significant effect on the load repetition number but
the increase of the graphite content with aging time has a
significant ef- fect on the load repetition number.
The variation of load repetition number versus graphite content for
original and aged mixtures are giv- en in Figure 12. Here, it can
be said that graphite-added samples are more aged, in other words,
they are more affected from aging. However, graphite-added mixtures
which take more load repetition number than the pure mixture in the
fatigue test will be resistant to repeated loads of traffic for a
longer time without cracking at me- dium temperatures. The curves
are become upright and become decumbent at the left and the right
side of the 15% graphite content at the aged situations. Hence the
15% graphite content can be assumed as the most effec- tive value
in terms of fatigue life.
In this study, the effects of graphite on mechanical fea- tures of
stone mastic asphalt pavement were researched. Mechanical tests
such as Marshall stability and flow, indi- rect tensile stiffness
modulus and indirect tensile fatigue tests were applied to
bituminous mixtures at three differ- ent proportions of graphite by
weight 10%, 15% and 20% of bitumen. It was determined that there is
no significant difference in mechanic properties of graphite added
mix- tures compared to the pure mixture at the unaged condi- tion.
The aging time considerably effects the performance
of pure and graphite added mixtures. The area under the
stress-deformation curves of aged mixtures indicates an improved
ability to absorb the elastic energy, at medium temperatures. After
15% graphite content the aging time lose its significance in terms
of stiffness modulus. The fa- tigue test results are also similar
to the stiffness modulus’ test results. While the load repetition
number of all mix- ture closes each other, graphite added mixture
exhibits a superior performance after aging. Effects of aging time
on load repetition number are more pronounced after the 15%
graphite content. G10, G15 and G20 mixtures have 7%, 65% and 78%
higher load repetition number com- pared to the pure mixture after
3-week aging condition.
Finally, it was found, 15% graphite content is an ef- fective ratio
when considering the elastic response, the absorbed energy, the
deformation behavior after the ini- tial crack and load repletion
number induced to deteriora- tion. According to these results,
graphite generally used for improving the thermal properties in
literature were also determined to contribute to mechanical
properties of mixtures at medium temperatures.
This research was supported by FUBAP (Firat University Scientific
Research Projects Unit) under the project num- ber MF 16.37 for
which the authors are greatly thankful. The findings and
evaluations of the results of this study are not the official views
References ASTM C 131 Standard Test Method for Resistance to
dation of Small-Size Coarse Aggregate by Abrasion and Impact in the
Los Angeles Machine. ASTM International, 2014.
ASTM C 88 Standard Test Method for Soundness of Aggregates by Use
of Sodium Sulfate or Magnesium Sulfate. ASTM International, 2013.
ASTM D 4791 Standard Test Method for Flat Particles, Elon- gated
Particles, or Flat and Elongated Particles in Coarse Aggregate.
ASTM International, 2010.
https://doi.org/10.1520/D4791-10 ASTM C127 Standard Test Method for
Relative Density (Spe-
cific Gravity) and Absorption of Coarse Aggregate. ASTM
International, 2015. https://doi.org/10.1520/C0127-15
Fig. 11. The load repetition number-deformation relation of the
Fig. 12. The load repetition number-graphite ratio relation of the
1020 B. V. Kök et al. Effects of graphite on mechanical properties
of stone mastic asphalt pavement
ASTM C128 Standard Test Method for Relative Density (Spe- cific
Gravity) and Absorption of Fine Aggregate. ASTM International,
ASTM D854 Standard Test Methods for Specific Gravity of Soil Solids
by Water Pycnometer. ASTM International, 2014.
Aghazadeh Dokandari, P.; Oner, J.; Topal, A.; Sengoz, B. 2014. A
laboratory study of an organic warm mix asphalt ad- ditive on aging
characteristics of bituminous mixtures, Pamukkale University
Journal Engineering Science 20: 332–337.
Austroads Technical Report. 2002. Stone mastic asphalt surfac- ing.
AAP asphalt guide.
Brainas, J.; Sivileviius, H.; Virbickas, R. 2013. Dependence of SMA
mixture and its bituminous binder properties on bitumen batching
system, mixing time and temperature on asphalt mixing plant,
Journal of Civil Engineering and Management 19(6): 862–872.
https://doi.org/10.3846/13923730.2013.843587 BS DD 213:1993 Method
for determination of the indirect tensile
stiffness modulus of bituminous mixtures. BSI Group, 1993. Chen,
J.; Wang, H.; Li, M.; Li, L. 2016. Evaluation of pave-
ment responses and performance with thermally modified asphalt
mixture, Materials and Design 111: 88–97.
https://doi.org/10.1016/j.matdes.2016.08.085 Dong, Y.; Tan, Y.
2011. Mix design and performance of crumb
rubber modified asphalt SMA, in GeoHunan International Conference
2011, 9–11 June 2011, Hunan, China.
https://doi.org/10.1061/47623(402)10 Du, Y.; Wang, S. 2015.
Oriented heat release in asphalt pave-
ment induced by high-thermal-conductivity rods, Applied Thermal
Engineering 90: 424–431.
https://doi.org/10.1016/j.applthermaleng.2015.07.026 Francken, L.
1998. Bituminous binders and mixes. Rilem
Reports. London and New York: E & FN Spon. Kim, Y.; Lim, J.;
Lee, M.; Kwon, S.; Hwang, S.; Lee, J. 2015.
Comprehensive evaluation of warm SMA using wax- based WMA additive
in Korea, Journal of Testing and Evaluation 43(5): 1230–1238.
https://doi.org/10.1520/JTE20130144 Kok, B. V.; Yilmaz, M.;
Akpolat, M. 2014. The effect of SBS and
wax modification on stability and stiffness of stone mastic
asphalt, Turkish Journal Science Technology 9: 56–72.
Liu, X.; Liu, W.; Wu, S.; Wang, C. 2014. Effect of carbon fillers
on electrical and road properties of conductive asphalt ma-
terials, Construction and Building Materials 68: 301–306.
Liu, Y.; Han, S.; Zhang, Z. 2012. Design and evaluation of gap-
graded asphalt rubber mixtures, Materials and Design 35: 873–877.
Lu, L.; Ao, Z.; He, Y.; Ding, Q.; Hu, S. 2008. Experimental study
on conductive asphalt concrete using steel slag as aggregate, in
the 1st International Conference on Micro- structure Related
Durability of Cementitious Composites, 2008, Nanjing, China,
Mamlouk, M.; Witczak, M.; Kaloush, K.; Hasan, N. 2005.
Determination of thermal properties of asphalt mixtures, Journal of
Testing and Evaluation 33(2): 118–126.
https://doi.org/10.1520/JTE12592 Moghaddam, T. B.; Karim, M. R.;
Syammaun, T. 2012. Dynamic
properties of stone mastic asphalt mixtures containing waste
plastic bottles, Construction and Building Materials 34: 236–242.
Mokhtari, A.; Nejad, F. M. 2012. Mechanistic approach for fiber and
polymer modified SMA mixtures, Construction and Building Materials
https://doi.org/10.1016/j.conbuildmat.2012.05.032 Pan, P.; Wu, S.;
Xiao, Y.; Wang, P.; Liu, X. 2014. Influence of
graphite on thermal properties and anti-aging properties of asphalt
binder, Construction and Building Materials 68: 220–226.
Radziszewski, P. 2007. Modified asphalt mixtures resistance to
permanent deformations, Journal of Civil Engineering and Management
Reed, J. 2010. Evaluation of the effects of aging on asphalt rubber
pavements: MSC thesis. Arizona State University.
Shatnawi, S. 2012. Superior aging characteristics of asphalt rub-
ber, in Asphalt Rubber Conference, 2012, 1–27.
Tongyan, P.; Yang, L.; Zhaoyang, W. 2012. Development of an
atomistic-based chemophysical environment for modeling asphalt
oxidation, Polymer Degradation and Stability 97: 2331–2339.
https://doi.org/10.1016/j.polymdegradstab.2012.07.032 TS EN
12697-34 Bituminous mixtures – Test methods for hot
mix asphalt – Part 34: Marshall. Turkish Standards In- stitution,
Xiao, F.; Amirkhanian, A. N.; Amirkhanian, S. N. 2011. Long- term
aging influence on rheological characteristics of as- phalt binders
containing carbon nanoparticles, Interna- tional Journal of
Pavement Engineering 12(6): 533–541.
Van Bijsterveld, W.; Houben, L. J.; Scarpas, A.; Molenear, A. A.
2001. Using pavement as solar collector: effect on pave- ment
temperature and structural response, Transportation Research
Record: Journal of the Transportation Research Board 1778: 140–148.
Wang, Y.; Sun, L.; Qin, Y. 2015. Aging mechanism of SBS modified
asphalt based on chemical reaction kinetics, Construction and
Building Materials 91: 47–56.
https://doi.org/10.1016/j.conbuildmat.2015.05.014 Yao, H.; Dai, Q.;
You, Z.; Ye, M.; Yap, Y. K. 2016. Rheologi-
cal properties, low-temperature cracking resistance, and optical
performance of exfoliated graphite nanoplate- lets modified asphalt
binder, Construction and Building Materials 113: 988–996.
https://doi.org/10.1016/j.conbuildmat.2016.03.152 Zoorob, S. E.;
Suparma, L. B. 2000. Laboratory design and in-
vestigation of properties of continuously graded Asphaltic concrete
containing recycled plastics aggregate replace- ment (Plastiphalt),
Cement and Concrete Composites 22(4): 233–242.
Baha Vural KÖK. Was born in Tukey in 1978. He is an associate
professor in civil engineering at Firat University where he teaches
highways design, bituminous materials, flexible asphalt pavements,
earthworks and other courses. His research interests include
bitumen modification, asphalt mixture design, performance of
asphalt pavement. He currently works on economic asphalt pavements
using waste materials. He has a lot of published manuscript at
Mehmet YILMAZ. Was born in Tukey in 1981. He is an associate
professor in civil engineering at Firat University where he teaches
highways design, experiments on bituminous materials, earthworks
and other courses. His work focuses on bitumen modi- fication,
asphalt mixture design, performance of asphalt pavement. He
currently works on self-treated asphalt pavements. He has a lot of
published manuscript at reputable journals.
Yunus ERKUS. Was born in Turkey in 1989. He is a PhD student and an
assistant professor at Firat University. He is a civil engineer.
His research interests focus on asphalt pavements.